The process of transforming hydromagnesite to magnesite is analysed in the context of the theory of solvent-mediated transformations. A series of experiments at 120, 150 and 180°C with different heating times was designed to determine, by powder X-ray diffraction, the amount of magnesite generated as a function of time. The aqueous-phase composition was monitored by inductively coupled plasma-mass spectrometry and carbonate alkalimetry. From the analytical data, the evolution of saturation indexes with respect to both phases was determined using the geochemical code PHREEQC. Finally, two different methods were applied to obtain the activation energy of the process and a TTT (Temperature-Transformation-Time) graph was constructed to define suitable conditions in which to obtain magnesite.
Global warming is an important issue worldwide and different possible remediation approaches are currently being discussed and developed. Among these approaches, geological storage of CO2 offers promise. The European Union is promoting significant advancements in this field, e.g. test injections of CO2, fully dissolved in water, into basaltic rocks (Matter et al., 2011; Gislason and Oelkers, 2014). The long-term stability of geological storage depends on the degree to which reactions between CO2, rocks and fluids are advantageous or detrimental (Oelkers and Gislason, 2010). One of the most important processes during the injection of CO2 into geological formations is the carbonation of (Mg,Fe,Ca)-silicates to give mineral phases such as magnesite – MgCO3, calcite – CaCO3, siderite – FeCO3, dolomite – CaMg(CO3)2 and carbonate solid solutions. Improving our understanding of the mineralization behaviour of anhydrous magnesium carbonates is a challenge related to the so-called “dolomite problem” (Weber, 1964; Ardvison and Mackenzie, 1999; Mackenzie and Andersson, 2013). Several studies (e.g. Sayles and Fyfe, 1973; Königsberger et al., 1999; Pokrovsky and Schott, 1999; Urosevic et al., 2012) have shown that it is impossible to precipitate anhydrous magnesium carbonate (magnesite) and this is attributed to the large dehydration energy associated with six molecules of H2O that constitute the solvation sphere of the aqueous Mg2+ ions. Because Mg2+ is smaller than Ca2+ and Fe2+, the charge density is greater in Mg2+ and the water molecules are more closely bound. The high-energy barrier that keeps the solvation molecules bound, does not allow for precipitation of magnesite at room temperature but favours crystallization of a series of hydrated carbonates and hydroxycarbonates (Pokrovsky et al., 1999; Hänchen et al., 2008; Saldi et al., 2009; Bénézeth et al., 2011) barringtonite MgCO3·2H2O, nesquehonite MgCO3·3H2O, lansfordite MgCO3·5H2O, hydromagnesite Mg5(CO3)4(OH)2·4H2O, dypingite Mg5(CO3)4(OH)2·5H2O, and artinite Mg2CO3(OH)2·3H2O. Recent studies of non-aqueous solvents (Xu et al., 2013) reconsider this hypothesis and indicate a strained accommodation of the CO3 group in the rhombohedral magnesite scheme that could inhibit the nucleation of magnesite at low temperatures.
The present study deals with the solvent-mediated transformation (Cardew and Davey, 1985) of hydromagnesite to magnesite during heating cycles over a range of temperature (120–180°C) in excess of the boiling point of water. For the three temperatures under investigation (120, 150 and 180°C) the transformation of hydromagnesite to magnesite (Sandengen et al., 2008; Xing et al., 2010) is analysed by applying the Avrami theory to isothermal solvent-mediated processes (Prigiobbe and Mazzotti, 2013). The transformation kinetics and the activation energy of the process are estimated using the so-called “time to a given fraction” method (Putnis, 1992). Moreover, the experimental data are used to construct a Temperature-Transformation-Time (TTT) graph.
Methods and materials
The experiments were performed by mixing 104.6 g of a 0.225 molal MgCl2 solution and 102.4 g of a 0.228 molal Na2CO3 solution. Analytical-grade chemicals (Panreac) and ultrapure water (MilliQ) were used in both cases. The two solutions were mixed in a PTFE (Polytetrafluoroethylene) vessel with a total volume of 304 ml and a diameter ∅vessel = 6.4 cm. Finally, 28 g of ultrapure water was added to the reaction vessel in order to obtain a volume-filling factor of 75% and a total, initial concentration of the reactants [Mg]T = [C(IV)]T ≈ 0.1 mol/kgw. The PTFE vessel was then inserted into a stainless steel high-pressure reactor (Berghof, BR-300) and placed in a heating block. The reactor is equipped with a temperature controller (Berghof, BDL-3000), a precision manometer, and magnetic stirring (impeller diameter ∅imp = 5 cm).
The reactor was heated and kept at the target temperature under continuous stirring (250 rpm) for defined periods of time. The two first columns (temperature and time) in Table 1 summarize the experiments performed. The experimental pressure is not displayed but was measured to be 9, 4 and 2 bars for 180, 150 and 120°C, respectively. After the corresponding reaction period, both heating and stirring were switched off, the solutions were extracted from the reactor, filtered (Ø = 0.45 μm, Pall Corporation), and analysed for magnesium (inductively coupled plasma-mass spectrometry – ICP-MS; HP 7500c Agilent), carbonate alkalinity (Crison Compact Titrator) and pH. The solid precipitates were dried at 30°C and characterized by powder X-ray diffraction (PXRD) (PANalytical X'Pert Pro) and scanning electron microscopy (SEM) imaging (JEOL-6610LV). The proportion (wt.%) of the different phases obtained in each precipitate was determined using the Rietveld quantitative-analysis tool implemented in the program X'Pert HighScore Plus version 1.0 (PANalytical). Speciation and saturation indices of the aqueous solutions were calculated from the analytical data using the geochemical code PHREEQC version 22.214.171.12438 (Parkhurst and Appelo, 2013).
Results and discussion
Figure 1 shows the typical diffraction patterns obtained for pure hydromagnesite, magnesite and a mixture of both phases (50 wt.%) obtained at different reaction times in the 180°C series. The coexistence of both phases in the same precipitate is shown in the SEM image in Figure 1, where the typical rhombohedral shape of the magnesite crystals (∅ ≈ 10 μm) can be observed. The evolution is similar in all of the series but the kinetics increase with running temperature. Although the initial precipitate formed at room temperature is a mixture of hydromagnesite and minor amounts of other Mg-carbonate hydrates, when the target temperature is reached, only hydromagnesite remains. During the reaction process no minerals other than magnesite and hydromagnesite were detected. The experimental data are compiled in Table 1, which displays as a function of the reaction time: (1) the wt.% of magnesite (Mgs) and hydromagnesite (Hmgs) in the precipitate; (2) the total aqueous concentration of magnesium [Mg]T; (3) the amount of magnesium precipitated Mg↓, and the molar fraction of magnesite. Note that all these compositions were measured after each heating cycle, when the system was back to 25°C.
Note that the amount of magnesite (Mgs, moles) in the precipitate increases significantly as the reaction proceeds. Such an increase correlates with a decrease in the amount of hydromagnesite (Hmgs, moles) and demonstrates the probable coupling between both processes. During the process the total amount of dissolved magnesium [Mg]T decreases by one order of magnitude, which is a consequence of the lower solubility of magnesite in comparison to hydromagnesite at the working temperatures. There is a transfer of magnesium from the aqueous to the solid phase and, therefore, the total amount of magnesium precipitated (Mg↓) increases as time goes by. The decrease in alkalinity is concomitant as both the total inorganic carbon (TIC) and the proportion of dissociated H2CO3 can be expected to decrease during precipitation of carbonates in a closed reactor. Figure 2 shows the evolution of the saturation indices (SI) with respect to both phases (see next section) in the case of the 180°C series. Both indices decrease during the precipitation-aging process. However, whereas magnesite slowly approaches equilibrium (SI = 0) from positive values, the saturation index with respect to hydromagnesite becomes negative. Clearly the progress of the reaction involves hydromagnesite dissolution and magnesite growth until the system reaches equilibrium with the stable, magnesite phase.
Hydrodynamics in the reaction vessel
At the beginning of the experiment the aqueous solution is supersaturated with respect to both phases (see Fig. 2). Note that although the saturation index with respect to magnesite is smaller than the saturation index with respect to hydromagnesite, the solubility of magnesite is lower than the solubility of hydromagnesite (S± (Mgs) = (Mgs) ≈ 9.38610−5 and S± (Hmgs) = (Hmgs) ≈ 3.12 × 10−4).
In fact, magnesite is the stable phase throughout the temperature range studied. As shown in Fig. 3, an aqueous solution at equilibrium with magnesite is undersaturated (SI < 0) with respect to hydromagnesite. However, in the initial solution, hydromagnesite precipitates metastably, which can be explained by its lower degree of dehydration. The precipitation of hydromagnesite continues until nucleation of magnesite occurs. At high temperature there is more chance of the Mg-solvation energy barrier being surpassed and the probability of nucleation of the anhydrous carbonate increases. When magnesite nucleation occurs the metastable hydromagnesite phase is near equilibrium with the aqueous solution, which is still supersaturated with respect to magnesite. Nucleation and growth of magnesite further decreases the activity of the aqueous Mg2+ ions and the solution becomes undersaturated with respect to hydromagnesite, which starts to dissolve. As a result, the metastable phase transforms into the stable phase through a dissolution-crystallization process.
Equation 7 represents the driving force for the solvent-mediated transformation of one mole of hydromagnesite to magnesite. For example, for the aqueous-solution composition obtained after 280 min of reaction a 180°C, ΔGtransf ≈ −244.2 kJ·mol−1, which illustrates the strong tendency of hydromagnesite to transform to magnesite at that temperature.
In practice, a linear fitting of the experimental values closer to YMgs = 0.5 allows interpolation of the time (t0.5) at which half of the final moles of magnesite were precipitated. Plotting lnt0.5 on the ordinate vs. 1/T on the abscissa, Ea/R is given by the slope of the corresponding linear fitting function (Fig. 5b). Here, the ‘time to a given fraction method’ gives a value of 93.3 kJ·mol−1 for the activation energy of the transformation of hydromagnesite to magnesite (see Table 4). The difference from the previous value is not surprising. In fact, this second method has the advantage of avoiding the strong dependence of the ‘kinetic constant’ method with respect to the function used to calculate the rate constant.
A suitable way to give kinetic information is the experimental determination of Temperature-Transformation-Time (TTT) diagrams. While TTT diagrams are commonly used in material and mineral sciences (Putnis, 1992) to deal with sub-solidus phase transformations, to our knowledge they have only been applied to coupled dissolution-crystallization processes in the case of the pseudomorphic replacement of leucite by analcime (Putnis et al., 2007). In the present study, a preliminary diagram from the experimental data compiled on Table 1 has been determined. The values of t0.05 and t0.95 corresponding to the three temperatures studied in this work were interpolated – the result is shown in Fig. 5c. Given that the transformation rate increases with increasing temperature, the diagrams cannot be expected to have the typical ‘C’ shape. The shape is similar to the diagrams of transformations that take place with rising temperature. These diagrams are particularly relevant to metamorphic processes because they allow us to determine if a given transformation will take place during a heating cycle. Reaching a high temperature is not sufficient for the transformation to occur in the case of a short heating period. In contrast, the transformation can occur at lower temperatures maintained for a prolonged time. The diagram in Fig. 5c could have a similar application as illustrated by the hypothetical heating cycles displayed in the graph. With this in mind, additional data for other temperatures should be obtained.
Conclusions and future work
The aim of the present study was to investigate the transformation of a hydrated magnesium carbonate phase to an anhydrous magnesium carbonate. A series of experiments at 120, 150 and 180°C with different heating times was performed to monitor the amount of magnesite generated (and hydromagnesite removed) as a function of time. According to the experimental results, the transformation can be considered a replacement (dissolution-precipitation) process. The activation energy calculated is an estimate of the energetic barrier that hinders the transformation of hydromagnesite into the thermodynamically stable magnesite phase as established from TST theory. Future efforts will attempt to determine the lowest temperature that allow the transformation to take place, and could help to solve the problems associated with the formation of anhydrous MgCO3. Although the present results allow us to discard transformation mechanisms other than dissolution-precipitation, the coupling between both processes will be investigated further by 18O isotope tracing between the aqueous solution and the precipitate (Ruiz-Agudo et al., 2014). Attempts will also be made to understand the mechanisms underlying the activation energy barrier for such a transformation and particularly the role of the mass-transfer effectiveness.
This work was supported by Marie Curie Initial Training Network “Geologic Carbon Storage” (European Commission, FP7-People-ITN-CO2-REACT-317235). The authors acknowledge Dr Christine V. Putnis and two anonymous reviewers for their insightful comments which helped to make a better and clearer manuscript. They also thank the editors for their comments and suggestions.